Lecture 7: Extrinsic semiconductors  Fermi level


 Isabella Woods
 4 years ago
 Views:
Transcription
1 Lecture 7: Extrinsic semiconductors  Fermi level Contents 1 Dopant materials 1 2 E F in extrinsic semiconductors 5 3 Temperature dependence of carrier concentration Low temperature regime (T < T s ) Medium temperature regime (T s < T < T i ) Dopant materials Typical doping concentrations in semiconductors are in ppm (10 6 ) and ppb (10 9 ). This small addition of impurities can cause orders of magnitude increase in conductivity. The impurity has to be of the right kind. For Si, ntype impurities are P, As, and Sb while ptype impurities are B, Al, Ga, and In. These form energy states close to the conduction and valence band and the ionization energies are a few tens of mev. Ge lies the same group IV as Si so that these elements are also used as impurities for Ge. The ionization energy data ntype impurities for Si and Ge are summarized in table 1. The ionization energy data for ptype impurities for Si and Ge is summarized in table 2. The dopant ionization energies for Ge are lower than Si. Ge has a lower band gap (0.67 ev ) compared to Si (1.10 ev ). Also, the Table 1: Ionization energies in mev for ntype impurities for Si and Ge. Typical values are close to room temperature thermal energy. Material P As Sb Si Ge
2 Table 2: Ionization energies in mev for ptype impurities. Typical values are comparable to room temperature thermal energy. Material B Al Ga In Si Ge relative permittivity for Ge is higher (ɛ r = 16) compared to Si (ɛ r = 11.9) and the effective masses for electron and holes are also different. The ionization energies for dopants in Si and Ge are represented in the band diagram schematically in figure 1. GaAs is a commonly used compound semiconductor. It is a IIIV semiconductor with predominantly covalent bonding, with some ionic character. Doping is done by substitution and there are a number of possibilities for GaAs, as seen from the periodic table shown in figure 2. For n type doping As (group V) can be replaced by elements from group VI. These have an extra electron and can act as donors. Similarly, for p type doping Ga (group III) can be replaced by group II elements, which act as acceptors. Si in group IV can act as both donor and acceptor, depending on where the Si atom is substituted. This is called amphoteric doping. It is hard to control the location of Si in the lattice to get a specific type of doping. Ionization energies of some common dopants in GaAs are shown in figure 3. Donors are located close to the conduction band and acceptors close to the valence band. Si impurity levels can be close to either, depending on whether it is substituted for Ga or As. Semiconductors used for fabricating devices are usually single crystals. This is because polycrystalline materials have defect states due to presence of grain boundaries. These defects states are located in the band gap and can modify the conductivity. There are two types of defect states 1. Shallow states  these are located close the band edges and can act as sources of electrons and holes. Common example is the dopants. 2. Deep states  these are located close to the center of the band gap, see figures 1 and3 for examples of both. Deep states can act as traps for charge carriers and reduce the conductivity. Film growth techniques can also introduce defects in a material, which can affect the conductivity. ZnO is a wide band gap semiconductor with E g of 3.4 ev. Thin films of ZnO growth by conventional vapor deposition or solution growth techniques are ntype because of the presence of Zn interstitials and O vacancies. Thus, it is very hard to get ptype ZnO because of the presence of these defects. 2
3 Figure 1: Ionization energies of dopants in Si and Ge. The gap center represents approximately the intrinsic Fermi level. Dopants located close to the band edges can be easily ionized and are called shallow states while those located closer to the gap center are called deep states. Adapted from Physics of semiconductor devices  S.M. Sze. 3
4 Figure 2: Portion of the periodic table around Ga and As (groups III and V). Elements from groups II  VI, can act as dopants. Source UseAPeriodicTable.htm Figure 3: Ionization energies of dopants in GaAs. Group II elements act as acceptors and group VI elements act as donors. Si can substitute in either Ga or As site,though Si as a ntype dopant (Ga substitution) has a lower energy. Adapted from Physics of semiconductor devices  S.M. Sze. 4
5 2 E F in extrinsic semiconductors In an intrinsic semiconductor, the Fermi level is located close to the center of the band gap. Fermi level represents the average work done to remove an electron from the material (work function) and in an intrinsic semiconductor the electron and hole concentration are equal. In an extrinsic semiconductor, with the dopants fully ionized, there is an imbalance in the electron and hole concentration. This in turn is reflected in the Fermi level position being shifted from the center of the band gap towards either the conduction band or valence band depending on the type of dopant. In an ntype semiconductor the electron concentration (n) is related to the position of the Fermi level (E F n ) by n = N c exp[ (E c E F n ) ] (1) k B T Equation 1 can be modified for an intrinsic semiconductor, where the Fermi level is close to center of the band gap (E F i ). n i = N c exp[ (E c E F i ) ] (2) k B T Manipulating equations 1 and 2, gives the Fermi level position in the ntype extrinsic semiconductor with respect to the intrinsic Fermi level E F n E F i = k B T ln( n n i ) (3) For an ntype semiconductor with N d donors which are fully ionized, n = N d when N d n i, so that the Fermi level is shifted above the center of the band gap, closer to the conduction band. For Si with N d = cm 3 and n i = cm 3, using equation 3, E F n is 0.25 ev above E F i. A similar argument can be used for ptype semiconductors, where the hole concentration is higher than the electron concentration. The Fermi level position (E F p ) is given by E F p E F i = k B T ln( p n i ) (4) For a ptype semiconductor with N a donors which are fully ionized, p = N a when N a n i, so that the Fermi level is shifted below the center of the band gap, closer to the valence band. The Fermi level position with carrier type and concentration for Si is summarized in figure 4. 5
6 Figure 4: E F position in Si, with doping type and concentration. The donor and acceptor concentration was varied from to cm 3 in steps of 10 and the temperature was varied from 200 to 450 K. The dotted line in the center represents E F i, which is approximately E g /2 at room temperature. For the calculation the variation of E F i with temperature was also considered. The plot was generated using MATLAB. 3 Temperature dependence of carrier concentration In an intrinsic semiconductor, the source of electrons and holes are the valence and conduction band. The carrier concentration depends exponentially on the band gap, given by n i = N c N v exp( E g 2k B T ) (5) A plot of n i vs. T is shown in figure 5. The plot is approximately a straight line, with the slope depending on the band gap. In an extrinsic n typesemiconductor, there are two sources for the electrons (same arguments are valid for ptype semiconductors) 1. The donor energy levels close to conduction band. This has an ionization energy mev. 2. The valence band of the semiconductor, with ionization energy ev. Because of the vast difference in the ionization energies for the two sources they operate in different temperature regimes, so that it is possible to understand the temperature behavior of the extrinsic semiconductors by dividing into different regimes 6
7 Figure 5: Carrier concentration vs. inverse temperature for three intrinsic semiconductors, Ge, Si, and GaAs. There is a single line with a constant slope, given by the band gap of the semiconductor. The plot was generated using MATLAB and the dotted line represents room temperature. 3.1 Low temperature regime (T < T s ) At absolute zero there are no ionized carriers. Valence band is full and the donor level is full and conduction band is empty. As temperature is increased, electrons are excited from the valence band and the donor level to the conduction band. But since the valence band ionization energy is of the order of ev, at low temperature the number of electrons excited from it are negligible compared to the electrons from the donor level. So the valence band contribution can be ignored and only electrons from the donor level are excited to the CB. This regime is called ionization regime and extends up to a temperature until all the donor electrons are ionized. The electron concentration (in CB), in the ionization regime, is given by n = ( 1 2 N c N d ) exp( E 2k B T ) (6) E is the ionization energy of the donor level i.e. the energy difference between the donor level and the conduction band. The 1 enters equation 6 2 because the donor levels are localized and can accommodate only one electron instead of two like a regular energy state. It is possible to define a saturation temperature (T s ) based on equation 6. The saturation temperature is defined as the temperature where n = 0.9N d where N d is the donor concentration. This corresponds to 90% ionization. Consider Si with N d of cm 3. Take N c to be independent of temperature and equal to cm 3. For As, E is ev. Then, using 7
8 equation 6 the saturation temperature, T s, is 32 K. The actual value (taking temperature dependence of N c ) is around 60 K, which is still much lower than room temperature. This means that the donor atoms (and similarly the acceptor atoms) are fully ionized at room temperature so that we are justified in equating the electron concentration (hole concentration) to the donor concentration (acceptor concentration). 3.2 Medium temperature regime (T s < T < T i ) Above the saturation temperature the donor levels are completely ionized so that n = N d. As temperature keeps increasing there comes a temperature when the electrons from the valence band (intrinsic carriers) becomes comparable in concentration to N d. This temperature is called the intrinsic temperature, T i. Above this temperature the semiconductor behaves as intrinsic. T i is defined as the temperature when n = 1.1 N d. This corresponds to 110% ionization. Between T s and T i the majority carrier concentration changes from 90% to 110% N d, so the variation in concentration is only 20% overall. The intrinsic temperature for Si can be calculated using the equation for intrinsic semiconductors. When n = 1.1 N d the hole concentration, p, can be calculated using a charge balance equation. n = p + N d (7) So, p = 0.1 N d. Using the law of mass action n 2 i = np, the intrinsic carrier concentration is 0.33 N d. This corresponds to a temperature of 526 K, which is the intrinsic temperature. Thus there is a temperature regime, from 60 K K, where the majority carrier concentration is nearly a constant. The majority carrier concentration vs. temperature is plotted in figure 6. There are 3 regions from the plot. A ionization regime at low temperature, a saturation regime where the electron concentration is nearly a constant, and a intrinsic regime where the semiconductor behaves like an intrinsic semiconductor. In Si, this saturation regime is around room temperature so that the carrier concentration is a constant and independent of temperature. Thus doping in a semiconductor has 2 functions 1. It increases the conductivity by preferentially increasing either electron or hole concentration. The conductivity can be precisely tuned by controlling the type and amount of dopant. 2. The majority carrier concentration is a constant and temperature independent (near room temperature) so that small temperature variations 8
9 Figure 6: Majority carrier concentration vs. inverse temperature for an extrinsic semiconductor. In the ionization regime, donor atoms are partially ionized. Then in the saturation regime where donors are fully ionized and carrier concentration is a constant. Finally, at high temperatures there is the intrinsic regime where it behaves like an intrinsic semiconductor. The temperatures corresponding to these depend on the donor concentration. The plot was generated in MATLAB with a donor concentration of cm 3. The vertical dotted line marks room temperature. 9
10 will not change the conductivity. Thus, electrical devices can be formed with very little variation in their electrical properties during normal operating temperatures. 10
Lecture 1. OUTLINE Basic Semiconductor Physics. Reading: Chapter 2.1. Semiconductors Intrinsic (undoped) silicon Doping Carrier concentrations
Lecture 1 OUTLINE Basic Semiconductor Physics Semiconductors Intrinsic (undoped) silicon Doping Carrier concentrations Reading: Chapter 2.1 EE105 Fall 2007 Lecture 1, Slide 1 What is a Semiconductor? Low
More informationEECS130 Integrated Circuit Devices
EECS130 Integrated Circuit Devices Professor Ali Javey 8/30/2007 Semiconductor Fundamentals Lecture 2 Read: Chapters 1 and 2 Last Lecture: Energy Band Diagram Conduction band E c E g Band gap E v Valence
More informationCh. 2: Energy Bands And Charge Carriers In Semiconductors
Ch. 2: Energy Bands And Charge Carriers In Semiconductors Discrete energy levels arise from balance of attraction force between electrons and nucleus and repulsion force between electrons each electron
More informationSemiconductors 1. Explain different types of semiconductors in detail with necessary bond diagrams. Intrinsic semiconductors:
Semiconductors 1. Explain different types of semiconductors in detail with necessary bond diagrams. There are two types of semi conductors. 1. Intrinsic semiconductors 2. Extrinsic semiconductors Intrinsic
More informationIntroduction to Engineering Materials ENGR2000. Dr.Coates
Introduction to Engineering Materials ENGR2000 Chapter 18: Electrical Properties Dr.Coates 18.2 Ohm s Law V = IR where R is the resistance of the material, V is the voltage and I is the current. l R A
More informationLecture 3b. Bonding Model and Dopants. Reading: (Cont d) Notes and Anderson 2 sections
Lecture 3b Bonding Model and Dopants Reading: (Cont d) Notes and Anderson 2 sections 2.32.7 The need for more control over carrier concentration Without help the total number of carriers (electrons and
More informationEE 346: Semiconductor Devices. 02/08/2017 Tewodros A. Zewde 1
EE 346: Semiconductor Devices 02/08/2017 Tewodros A. Zewde 1 DOPANT ATOMS AND ENERGY LEVELS Without help the total number of carriers (electrons and holes) is limited to 2ni. For most materials, this is
More informationElectrons, Holes, and Defect ionization
Electrons, Holes, and Defect ionization The process of forming intrinsic electronhole pairs is excitation a cross the band gap ( formation energy ). intrinsic electronic reaction : null e + h When electrons
More informationLN 3 IDLE MIND SOLUTIONS
IDLE MIND SOLUTIONS 1. Let us first look in most general terms at the optical properties of solids with band gaps (E g ) of less than 4 ev, semiconductors by definition. The band gap energy (E g ) can
More informationChemistry Instrumental Analysis Lecture 8. Chem 4631
Chemistry 4631 Instrumental Analysis Lecture 8 UV to IR Components of Optical Basic components of spectroscopic instruments: stable source of radiant energy transparent container to hold sample device
More informationEECS143 Microfabrication Technology
EECS143 Microfabrication Technology Professor Ali Javey Introduction to Materials Lecture 1 Evolution of Devices Yesterday s Transistor (1947) Today s Transistor (2006) Why Semiconductors? Conductors e.g
More informationA semiconductor is an almost insulating material, in which by contamination (doping) positive or negative charge carriers can be introduced.
Semiconductor A semiconductor is an almost insulating material, in which by contamination (doping) positive or negative charge carriers can be introduced. Page 2 Semiconductor materials Page 3 Energy levels
More informationPH575 Spring Lecture #19 Semiconductors: electrical & optical properties: Kittel Ch. 8 pp ; Ch. 20
PH575 Spring 2014 Lecture #19 Semiconductors: electrical & optical properties: Kittel Ch. 8 pp. 205214; Ch. 20 Simplified diagram of the filling of electronic band structure in various types of material,
More informationsmal band gap Saturday, April 9, 2011
small band gap upper (conduction) band empty small gap valence band filled 2s 2p 2s 2p hybrid (s+p)band 2p no gap 2s (depend on the crystallographic orientation) extrinsic semiconductor semimetal electron
More informationEE143 Fall 2016 Microfabrication Technologies. Evolution of Devices
EE143 Fall 2016 Microfabrication Technologies Prof. Ming C. Wu wu@eecs.berkeley.edu 511 Sutardja Dai Hall (SDH) 11 Evolution of Devices Yesterday s Transistor (1947) Today s Transistor (2006) 12 1 Why
More informationReview of Semiconductor Fundamentals
ECE 541/ME 541 Microelectronic Fabrication Techniques Review of Semiconductor Fundamentals Zheng Yang (ERF 3017, email: yangzhen@uic.edu) Page 1 Semiconductor A semiconductor is an almost insulating material,
More informationCME 300 Properties of Materials. ANSWERS: Homework 9 November 26, As atoms approach each other in the solid state the quantized energy states:
CME 300 Properties of Materials ANSWERS: Homework 9 November 26, 2011 As atoms approach each other in the solid state the quantized energy states: are split. This splitting is associated with the wave
More informationLecture 2  Carrier Statistics in Equilibrium. September 5, 2002
6.720J/3.43J Integrated Microelectronic Devices Fall 2002 Lecture 21 Lecture 2 Carrier Statistics in Equilibrium Contents: September 5, 2002 1. Conduction and valence bands, bandgap, holes 2. Intrinsic
More informationCLASS 12th. Semiconductors
CLASS 12th Semiconductors 01. Distinction Between Metals, Insulators and SemiConductors Metals are good conductors of electricity, insulators do not conduct electricity, while the semiconductors have
More informationMTLE6120: Advanced Electronic Properties of Materials. Intrinsic and extrinsic semiconductors. Reading: Kasap:
MTLE6120: Advanced Electronic Properties of Materials 1 Intrinsic and extrinsic semiconductors Reading: Kasap: 5.15.6 Band structure and conduction 2 Metals: partially filled band(s) i.e. bands cross
More informationLecture 15: Optoelectronic devices: Introduction
Lecture 15: Optoelectronic devices: Introduction Contents 1 Optical absorption 1 1.1 Absorption coefficient....................... 2 2 Optical recombination 5 3 Recombination and carrier lifetime 6 3.1
More informationELECTRONIC I Lecture 1 Introduction to semiconductor. By Asst. Prof Dr. Jassim K. Hmood
ELECTRONIC I Lecture 1 Introduction to semiconductor By Asst. Prof Dr. Jassim K. Hmood SOLIDSTATE ELECTRONIC MATERIALS Electronic materials generally can be divided into three categories: insulators,
More informationSemiconductor physics I. The Crystal Structure of Solids
Lecture 3 Semiconductor physics I The Crystal Structure of Solids 1 Semiconductor materials Types of solids Space lattices Atomic Bonding Imperfection and doping in SOLIDS 2 Semiconductor Semiconductors
More informationBasic cell design. Si cell
Basic cell design Si cell 1 Concepts needed to describe photovoltaic device 1. energy bands in semiconductors: from bonds to bands 2. free carriers: holes and electrons, doping 3. electron and hole current:
More informationCHAPTER 2: ENERGY BANDS & CARRIER CONCENTRATION IN THERMAL EQUILIBRIUM. M.N.A. Halif & S.N. Sabki
CHAPTER 2: ENERGY BANDS & CARRIER CONCENTRATION IN THERMAL EQUILIBRIUM OUTLINE 2.1 INTRODUCTION: 2.1.1 Semiconductor Materials 2.1.2 Basic Crystal Structure 2.1.3 Basic Crystal Growth technique 2.1.4 Valence
More informationEE 346: Semiconductor Devices
EE 346: Semiconductor Devices Lecture  6 02/06/2017 Tewodros A. Zewde 1 DENSTY OF STATES FUNCTON Since current is due to the flow of charge, an important step in the process is to determine the number
More informationDirect and Indirect Semiconductor
Direct and Indirect Semiconductor Allowed values of energy can be plotted vs. the propagation constant, k. Since the periodicity of most lattices is different in various direction, the Ek diagram must
More informationNote that it is traditional to draw the diagram for semiconductors rotated 90 degrees, i.e. the version on the right above.
5 Semiconductors The nearly free electron model applies equally in the case where the Fermi level lies within a small band gap (semiconductors), as it does when the Fermi level lies within a band (metal)
More informationCharge Carriers in Semiconductor
Charge Carriers in Semiconductor To understand PN junction s IV characteristics, it is important to understand charge carriers behavior in solids, how to modify carrier densities, and different mechanisms
More informationVariation of Energy Bands with Alloy Composition E
Variation of Energy Bands with Alloy Composition E 3.0 E.8.6 L 0.3eV Al x GaAs AlAs 1 xas 1.43eV.16eV X k.4 L. X.0 X 1.8 L 1.6 1.4 0 0. 0.4 0.6 X 0.8 1 1 Carriers in intrinsic Semiconductors Ec 4º 1º
More informationThe Semiconductor in Equilibrium
Lecture 6 Semiconductor physics IV The Semiconductor in Equilibrium Equilibrium, or thermal equilibrium No external forces such as voltages, electric fields. Magnetic fields, or temperature gradients are
More informationLecture 2 Electrons and Holes in Semiconductors
EE 471: Transport Phenomena in Solid State Devices Spring 2018 Lecture 2 Electrons and Holes in Semiconductors Bryan Ackland Department of Electrical and Computer Engineering Stevens Institute of Technology
More informationMat E 272 Lecture 25: Electrical properties of materials
Mat E 272 Lecture 25: Electrical properties of materials December 6, 2001 Introduction: Calcium and copper are both metals; Ca has a valence of +2 (2 electrons per atom) while Cu has a valence of +1 (1
More informationSEMICONDUCTOR PHYSICS
SEMICONDUCTOR PHYSICS by Dibyendu Chowdhury Semiconductors The materials whose electrical conductivity lies between those of conductors and insulators, are known as semiconductors. Silicon Germanium Cadmium
More informationGa and P Atoms to Covalent Solid GaP
Ga and P Atoms to Covalent Solid GaP Band Gaps in Binary Group IIIV Semiconductors Mixed Semiconductors Affect of replacing some of the As with P in GaAs Band Gap (ev) (nm) GaAs 1.35 919 (IR) GaP 2.24
More informationLecture 2. Semiconductor Physics. Sunday 4/10/2015 Semiconductor Physics 11
Lecture 2 Semiconductor Physics Sunday 4/10/2015 Semiconductor Physics 11 Outline Intrinsic bond model: electrons and holes Charge carrier generation and recombination Intrinsic semiconductor Doping:
More informationCLASS 1 & 2 REVISION ON SEMICONDUCTOR PHYSICS. Reference: Electronic Devices by Floyd
CLASS 1 & 2 REVISION ON SEMICONDUCTOR PHYSICS Reference: Electronic Devices by Floyd 1 ELECTRONIC DEVICES Diodes, transistors and integrated circuits (IC) are typical devices in electronic circuits. All
More informationLecture 2  Carrier Statistics in Equilibrium. February 8, 2007
6.720J/3.43J Integrated Microelectronic Devices Spring 2007 Lecture 21 Lecture 2 Carrier Statistics in Equilibrium Contents: February 8, 2007 1. Conduction and valence bands, bandgap, holes 2. Intrinsic
More informationSemiconductors. SEM and EDAX images of an integrated circuit. SEM EDAX: Si EDAX: Al. Institut für Werkstoffe der ElektrotechnikIWE
SEM and EDAX images of an integrated circuit SEM EDAX: Si EDAX: Al source: [Cal 99 / 605] M&D.PPT, slide: 1, 12.02.02 Classification semiconductors electronic semiconductors mixed conductors ionic conductors
More informationIntrinsic Semiconductors
Technische Universität Graz Institute of Solid State Physics Intrinsic Semiconductors ermi function f(e) is the probability that a state at energy E is occupied. f( E) 1 E E 1 exp kt B ermi energy The
More informationChapter 1 Overview of Semiconductor Materials and Physics
Chapter 1 Overview of Semiconductor Materials and Physics Professor Paul K. Chu Conductivity / Resistivity of Insulators, Semiconductors, and Conductors Semiconductor Elements Period II III IV V VI 2 B
More informationELEMENTARY BAND THEORY
ELEMENTARY BAND THEORY PHYSICIST Solid state band Valence band, VB Conduction band, CB Fermi energy, E F Bloch orbital, delocalized ndoping pdoping Band gap, E g Direct band gap Indirect band gap Phonon
More informationKATIHAL FİZİĞİ MNT510
KATIHAL FİZİĞİ MNT510 YARIİLETKENLER Kaynaklar: Katıhal Fiziği, Prof. Dr. Mustafa Dikici, Seçkin Yayıncılık Katıhal Fiziği, Şakir Aydoğan, Nobel Yayıncılık, Physics for Computer Science Students: With
More informationEXTRINSIC SEMICONDUCTOR
EXTRINSIC SEMICONDUCTOR EXTRINSIC SEMICONDUCTOR A semiconductor in which the impurity atoms are added by doping process is called Extrinsic semiconductor. The addition of impurities increases the carrier
More informationSemiconductors. Semiconductors also can collect and generate photons, so they are important in optoelectronic or photonic applications.
Semiconductors Semiconducting materials have electrical properties that fall between true conductors, (like metals) which are always highly conducting and insulators (like glass or plastic or common ceramics)
More informationDensity of states for electrons and holes. Distribution function. Conduction and valence bands
Intrinsic Semiconductors In the field of semiconductors electrons and holes are usually referred to as free carriers, or simply carriers, because it is these particles which are responsible for carrying
More informationIntroduction to Semiconductor Physics. Prof.P. Ravindran, Department of Physics, Central University of Tamil Nadu, India
Introduction to Semiconductor Physics 1 Prof.P. Ravindran, Department of Physics, Central University of Tamil Nadu, India http://folk.uio.no/ravi/cmp2013 Review of Semiconductor Physics Semiconductor fundamentals
More informationDiamond. Covalent Insulators and Semiconductors. Silicon, Germanium, Gray Tin. Chem 462 September 24, 2004
Covalent Insulators and Chem 462 September 24, 2004 Diamond Pure sp 3 carbon All bonds staggered ideal d(cc)  1.54 Å, like ethane Silicon, Germanium, Gray Tin Diamond structure Si and Ge: semiconductors
More informationECE 335: Electronic Engineering Lecture 2: Semiconductors
Faculty of Engineering ECE 335: Electronic Engineering Lecture 2: Semiconductors Agenda Intrinsic Semiconductors Extrinsic Semiconductors Ntype Ptype Carrier Transport Drift Diffusion Semiconductors
More informationEngineering 2000 Chapter 8 Semiconductors. ENG2000: R.I. Hornsey Semi: 1
Engineering 2000 Chapter 8 Semiconductors ENG2000: R.I. Hornsey Semi: 1 Overview We need to know the electrical properties of Si To do this, we must also draw on some of the physical properties and we
More informationn i exp E g 2kT lnn i E g 2kT
HOMEWORK #10 12.19 For intrinsic semiconductors, the intrinsic carrier concentration n i depends on temperature as follows: n i exp E g 2kT (28.35a) or taking natural logarithms, lnn i E g 2kT (12.35b)
More information2. Point Defects. R. KrauseRehberg
R. KrauseRehberg 2. Point Defects (Fcenter in NaCl) 2.1 Introduction 2.2 Classification 2.3 Notation 2.4 Examples 2.5 Peculiarities in Semiconductors 2.6 Determination of Structure and Concentration
More informationSemiconductor Physics. Lecture 3
Semiconductor Physics Lecture 3 Intrinsic carrier density Intrinsic carrier density Law of mass action Valid also if we add an impurity which either donates extra electrons or holes the number of carriers
More informationDetermination of properties in semiconductor materials by applying Matlab
Determination of properties in semiconductor materials by applying Matlab Carlos Figueroa. 1, Raúl Riera A. 2 1 Departamento de Ingeniería Industrial. Universidad de Sonora A.P. 5088, Hermosillo, Sonora.
More informationCrystal Properties. MS415 Lec. 2. High performance, high current. ZnO. GaN
Crystal Properties Crystal Lattices: Periodic arrangement of atoms Repeated unit cells (solidstate) Stuffing atoms into unit cells Determine mechanical & electrical properties High performance, high current
More informationChapter 2. Semiconductor Fundamentals
hapter Semiconductor Fundamentals.0 Introduction There are altogether 9 types of natural occurring elements, of which only few types are important in semiconductor physics and technology. They are the
More informationESE370: CircuitLevel Modeling, Design, and Optimization for Digital Systems
ESE370: CircuitLevel Modeling, Design, and Optimization for Digital Systems Lec 6: September 14, 2015 MOS Model You are Here: Transistor Edition! Previously: simple models (0 and 1 st order) " Comfortable
More informationAtoms? All matters on earth made of atoms (made up of elements or combination of elements).
Chapter 1 Atoms? All matters on earth made of atoms (made up of elements or combination of elements). Atomic Structure Atom is the smallest particle of an element that can exist in a stable or independent
More informationFirstHand Investigation: Modeling of Semiconductors
perform an investigation to model the behaviour of semiconductors, including the creation of a hole or positive charge on the atom that has lost the electron and the movement of electrons and holes in
More informationMark Lundstrom 2/10/2013. SOLUTIONS: ECE 606 Homework Week 5 Mark Lundstrom Purdue University (corrected 3/26/13)
SOLUIONS: ECE 606 Homework Week 5 Mark Lundstrom Purdue University corrected 6/13) Some of the problems below are taken/adapted from Chapter 4 in Advanced Semiconductor Fundamentals, nd. Ed. By R.F. Pierret.
More informationChapter 12: Semiconductors
Chapter 12: Semiconductors Bardeen & Shottky January 30, 2017 Contents 1 Band Structure 4 2 Charge Carrier Density in Intrinsic Semiconductors. 6 3 Doping of Semiconductors 12 4 Carrier Densities in Doped
More informationSolid State Electronics EC210 Arab Academy for Science and Technology AAST Cairo Fall Lecture 10: Semiconductors
Solid State Electronics EC210 Arab Academy for Science and Technology AAST Cairo Fall 2014 Lecture 10: Semiconductors Lecture Notes Prepared by: Dr. Amr Bayoumi, Dr. Nadia Rafat These PowerPoint color
More informationECE 442. Spring, Lecture 2
ECE 442 Power Semiconductor Devices and Integrated circuits Spring, 2006 University of Illinois at Chicago Lecture 2 Semiconductor physics band structures and charge carriers 1. What are the types of
More information3.23 Electrical, Optical, and Magnetic Properties of Materials
MIT OpenCourseWare http://ocw.mit.edu 3.23 Electrical, Optical, and Magnetic Properties of Materials Fall 2007 For information about citing these materials or our Terms of Use, visit: http://ocw.mit.edu/terms.
More informationSolid State Device Fundamentals
4. lectrons and Holes Solid State Device Fundamentals NS 45 Lecture Course by Alexander M. Zaitsev alexander.zaitsev@csi.cuny.edu Tel: 718 982 2812 4N101b 1 4. lectrons and Holes Free electrons and holes
More informationn N D n p = n i p N A
Summary of electron and hole concentration in semiconductors Intrinsic semiconductor: E G n kt i = pi = N e 2 0 Donordoped semiconductor: n N D where N D is the concentration of donor impurity Acceptordoped
More informationElectrical Properties
Electrical Properties Electrical Conduction R Ohm s law V = IR I l Area, A V where I is current (Ampere), V is voltage (Volts) and R is the resistance (Ohms or ) of the conductor Resistivity Resistivity,
More informationIntroduction into defect studies. in ceramic materials(iii) Structure, Defects and Defect Chemistry. Z. Wang. January 18, 2002
Introduction into defect studies in ceramic materials(iii) Structure, Defects and Defect Chemistry Z. Wang January 18, 2002 1. Mass, Charge and Site Balance The Schottky reactions for NaCl and MgO, respectively,
More informationKey Questions. ECE 340 Lecture 6 : Intrinsic and Extrinsic Material I 9/10/12. Class Outline: Effective Mass Intrinsic Material
9/1/1 ECE 34 Lecture 6 : Intrinsic and Extrinsic Material I Class Outline: Things you should know when you leave Key Questions What is the physical meaning of the effective mass What does a negative effective
More informationSemiconductor Physics
Semiconductor Physics Motivation Is it possible that there might be current flowing in a conductor (or a semiconductor) even when there is no potential difference supplied across its ends? Look at the
More informationECE 340 Lecture 6 : Intrinsic and Extrinsic Material I Class Outline:
ECE 340 Lecture 6 : Intrinsic and Extrinsic Material I Class Outline: Effective Mass Intrinsic Material Extrinsic Material Things you should know when you leave Key Questions What is the physical meaning
More informationChapter 12: Electrical Properties. RA l
Charge carriers and conduction: Chapter 12: Electrical Properties Charge carriers include all species capable of transporting electrical charge, including electrons, ions, and electron holes. The latter
More informationESE 372 / Spring 2013 / Lecture 5 Metal Oxide Semiconductor Field Effect Transistor
Metal Oxide Semiconductor Field Effect Transistor V G V G 1 Metal Oxide Semiconductor Field Effect Transistor We will need to understand how this current flows through Si What is electric current? 2 Back
More informationClassification of Solids
Classification of Solids Classification by conductivity, which is related to the band structure: (Filled bands are shown dark; D(E) = Density of states) Class Electron Density Density of States D(E) Examples
More informationElectrical material properties
Electrical material properties U = I R Ohm s law R = ρ (l/a) ρ resistivity l length σ = 1/ρ σ conductivity A area σ = n q μ n conc. of charge carriers q their charge μ their mobility μ depends on T, defects,
More informationV = IR or R = V I. R = ρ l A
Metals and Semiconductors Ram Seshadri MRL 2031, x6129, seshadri@mrl.ucsb.edu Electrical resistance and Ohm s Law: If an electric current I (units of A, Ampère) flows through a conductor with resistance
More informationSemiconductorDetectors
SemiconductorDetectors 1 Motivation ~ 195: Discovery that pn junctions can be used to detect particles. Semiconductor detectors used for energy measurements ( Germanium) Since ~ 3 years: Semiconductor
More informationDependence of Hole Concentration in ptype Silicon Solar Cell Wafers on Temperature and on Position within the Polycrystalline Ingot
Dependence of Hole Concentration in ptype Silicon Solar Cell Wafers on Temperature and on Position within the Polycrystalline Ingot H. Matsuura, T. Ishida, K. ishikawa. Fukunaga and T. Kuroda Department
More informationIntroductory Nanotechnology ~ Basic Condensed Matter Physics ~
Introductory Nanotechnology ~ Basic Condensed Matter Physics ~ Atsufumi Hirohata Department of Electronics Quick Review over the Last Lecture Classic model : DulongPetit empirical law c V, mol 3R 0 E
More informationUNIVERSITY OF CALIFORNIA College of Engineering Department of Electrical Engineering and Computer Sciences. Fall Exam 1
UNIVERSITY OF CALIFORNIA College of Engineering Department of Electrical Engineering and Computer Sciences EECS 143 Fall 2008 Exam 1 Professor Ali Javey Answer Key Name: SID: 1337 Closed book. One sheet
More informationMinimal Update of Solid State Physics
Minimal Update of Solid State Physics It is expected that participants are acquainted with basics of solid state physics. Therefore here we will refresh only those aspects, which are absolutely necessary
More informationV BI. H. Föll: kiel.de/matwis/amat/semi_en/kap_2/backbone/r2_2_4.html. different electrochemical potentials (i.e.
Consider the the band diagram for a homojunction, formed when two bits of the same type of semicondutor (e.g. Si) are doped p and ntype and then brought into contact. Electrons in the two bits have different
More informationFree Electron Model for Metals
Free Electron Model for Metals Metals are very good at conducting both heat and electricity. A lattice of in a sea of electrons shared between all nuclei (moving freely between them): This is referred
More information! Previously: simple models (0 and 1 st order) " Comfortable with basic functions and circuits. ! This week and next (4 lectures)
ESE370: CircuitLevel Modeling, Design, and Optimization for Digital Systems Lec 6: September 14, 2015 MOS Model You are Here: Transistor Edition! Previously: simple models (0 and 1 st order) " Comfortable
More information3. Semiconductor heterostructures and nanostructures
3. Semiconductor eterostructures and nanostructures We discussed before ow te periodicity of a crystal results in te formation of bands. or a 1D crystal, we obtained: a (x) x In 3D, te crystal lattices
More informationR measurements (resistivity, magnetoresistance, Hall). Makariy A. Tanatar
R measurements (resistivity, magnetoresistance, Hall). 590B Makariy A. Tanatar April 18, 2014 Resistivity Typical resistivity temperature dependence: metals, semiconductors Magnetic scattering Resistivities
More informationECE 250 Electronic Devices 1. Electronic Device Modeling
ECE 250 Electronic Devices 1 ECE 250 Electronic Device Modeling ECE 250 Electronic Devices 2 Introduction to Semiconductor Physics You should really take a semiconductor device physics course. We can only
More informationBasic Semiconductor Physics
6 Basic Semiconductor Physics 6.1 Introduction With this chapter we start with the discussion of some important concepts from semiconductor physics, which are required to understand the operation of solar
More informationElectronics The basics of semiconductor physics
Electronics The basics of semiconductor physics Prof. Márta Rencz, Gergely Nagy BME DED September 16, 2013 The basic properties of semiconductors Semiconductors conductance is between that of conductors
More informationUnit IV Semiconductors Engineering Physics
Introduction A semiconductor is a material that has a resistivity lies between that of a conductor and an insulator. The conductivity of a semiconductor material can be varied under an external electrical
More informationElectron Energy, E E = 0. Free electron. 3s Band 2p Band Overlapping energy bands. 3p 3s 2p 2s. 2s Band. Electrons. 1s ATOM SOLID.
Electron Energy, E Free electron Vacuum level 3p 3s 2p 2s 2s Band 3s Band 2p Band Overlapping energy bands Electrons E = 0 1s ATOM 1s SOLID In a metal the various energy bands overlap to give a single
More informationSpring 2010 MSE 111. Midterm Exam. Prof. Eugene E. Haller. University of California at Berkeley Department of Materials Science and Engineering
Spring 00 MS Midterm xam Prof. ugene. Haller University of California at Berkeley Department of Materials Science and ngineering 3/6/0, 9:40 am 80 minutes, 74 points total, 0 pages ame: SID: Problem 3
More informationChapter 1 Semiconductor basics
Chapter 1 Semiconductor basics ELECH402/CH1: Semiconductor basics 1 Basic semiconductor concepts Semiconductor basics Semiconductors, silicon and holeelectron pair Intrinsic silicon properties Doped
More informationESE370: CircuitLevel Modeling, Design, and Optimization for Digital Systems
ESE370: CircuitLevel Modeling, Design, and Optimization for Digital Systems Lec 6: September 18, 2017 MOS Model You are Here: Transistor Edition! Previously: simple models (0 and 1 st order) " Comfortable
More informationSemiconductor Device Physics
1 Semiconductor Device Physics Lecture 1 http://zitompul.wordpress.com 2 0 1 3 2 Semiconductor Device Physics Textbook: Semiconductor Device Fundamentals, Robert F. Pierret, International Edition, Addison
More informationSemiconductor Physics Problems 2015
Semiconductor Physics Problems 2015 Page and figure numbers refer to Semiconductor Devices Physics and Technology, 3rd edition, by SM Sze and MK Lee 1. The purest semiconductor crystals it is possible
More informationElectrical Resistance
Electrical Resistance I + V _ W Material with resistivity ρ t L Resistance R V I = L ρ Wt (Unit: ohms) where ρ is the electrical resistivity 1 Adding parts/billion to parts/thousand of dopants to pure
More informationECE 142: Electronic Circuits Lecture 3: Semiconductors
Faculty of Engineering ECE 142: Electronic Circuits Lecture 3: Semiconductors Agenda Intrinsic Semiconductors Extrinsic Semiconductors Ntype Ptype Carrier Transport Drift Diffusion Semiconductors A semiconductor
More informationDue to the quantum nature of electrons, one energy state can be occupied only by one electron.
In crystalline solids, not all values of the electron energy are possible. The allowed intervals of energy are called allowed bands (shown as blue and chessboard blue). The forbidden intervals are called
More informationSemiconductor Devices and Circuits Fall Midterm Exam. Instructor: Dr. Dietmar Knipp, Professor of Electrical Engineering. Name: Mat. Nr.
Semiconductor Devices and Circuits Fall 2003 Midterm Exam Instructor: Dr. Dietmar Knipp, Professor of Electrical Engineering Name: Mat. Nr.: Guidelines: Duration of the Midterm: 1 hour The exam is a closed
More information